The Saudi Dental Journal (2014) 26, 15–18
King Saud University
The Saudi Dental Journal www.ksu.edu.sa www.sciencedirect.com
Elastic modulus and ﬂexural strength comparisons of high-impact and traditional denture base acrylic resins Nour M. Ajaj-ALKordy *, Mohannad H. Alsaadi Department of Removable Prosthodontics, Faculty of Dental Medicine, Damascus University, Syria Received 13 June 2013; revised 5 November 2013; accepted 3 December 2013 Available online 19 December 2013
KEYWORDS Denture; Acrylic resin; Fracture; High-impact; Elastic modulus; Flexural strength
Abstract Background: Fractures of acrylic resin dentures are a common occurrence in clinical dentistry. The denture may be fractured accidentally when dropped or while in service in the mouth due to ﬂexural fatigue. Objectives: The aim of this study was to compare the elastic modulus and the ﬂexural strength between two heat-cured acrylic resins used in denture bases: a high-impact resin (Lucitone 199) and a traditional resin (Rodex). Materials and methods: Rectangular strips of Lucitone 199 and Rodex (10 samples each) were fabricated and stored in artiﬁcial saliva at 37 C for 2 weeks. The specimens were subjected to a three-point ﬂexural test. The data were statistically analysed with Student’s t-test (p 6 .05). Results: The high-impact acrylic resin had a lower elastic modulus (p = .000) and higher ﬂexural strength (p = .001) compared to the traditional acrylic resin. Conclusion: Within the limitations of this study, it can be concluded that the high-impact acrylic resin is a suitable denture base material for patients with clinical fracture of the acrylic denture. ª 2013 King Saud University. Production and hosting by Elsevier B.V. All rights reserved.
1. Introduction Polymethyl methacrylate (PMMA) resins are commonly used for the fabrication of denture bases, owing to their good aes* Corresponding author. Tel.: +963 112236154/52380, mobile: +963 933452380/944452380. E-mail address: [email protected]
(N.M. Ajaj-ALKordy). Peer review under responsibility of King Saud University.
Production and hosting by Elsevier
thetics, simple processing, and relative ease of repair (Cheng et al., 2010; Hirajima et al., 2009). However, insufﬁcient mechanical properties render them non-ideal (Seo et al., 2006). In particular, acrylic resin dentures are prone to fracture, which may occur by impact when the denture is outside the mouth, or while in service in the mouth due to ﬂexural fatigue as the denture base undergoes repeated masticatory loading (Johnston et al., 1981; Hirajima et al., 2009; Kelly, 1969). High ﬂexural strength is crucial to the success of denture wearing, as alveolar absorption is a gradual and irregular process that causes uneven prosthesis support (Diaz-Arnold et al., 2008). To ensure that the stresses encountered during biting
1013-9052 ª 2013 King Saud University. Production and hosting by Elsevier B.V. All rights reserved. http://dx.doi.org/10.1016/j.sdentj.2013.12.005
16 and mastication do not cause permanent deformation, the denture base material should exhibit a high elastic modulus (McCabe and Walls, 1998). Meng and Latta (2005) determined the Izod impact strength, ﬂexural strength, ﬂexural modulus, and yield distance for four denture resins (i.e., Lucitone 199, Fricke Hi-I, ProBase Hot, and Sledgehammer Maxipack). Among the tested resins, Lucitone 199 demonstrated the highest impact strength, ﬂexural strength, and yield distance (p < .05). Moreover, the ﬂexural modulus had an inverse relationship with the impact strength, ﬂexural strength, and yield distance. Diaz-Arnold et al. (2008) evaluated the ﬂexural strength of four PMMA acrylic resin materials (i.e., Diamond D, Fricke HI-I, Lucitone 199, Nature-Cryl Hi-Plus) and one urethane dimethacrylate material (i.e., Eclipse). The visible light-polymerized Eclipse resin demonstrated a greater ﬂexural strength than all of the PMMA heat-polymerized resins. Few studies have evaluated the stiffness and ﬂexural strength of high-impact resin. Therefore, the purpose of this paper was to evaluate the elastic modulus and ﬂexural strength of two heat-cured denture base acrylic resins: speciﬁcally, a high-impact resin (Lucitone 199) and a traditional resin (Rodex).
N.M. Ajaj-ALKordy, M.H. Alsaadi (m), and d is the specimen thickness (m) (Anusavice and Phillips, 2003). The elastic modulus (E, in MPa) was calculated by E = (P/db)/ (Dl/l), where Dl is the increase in specimen length (m) (Anusavice and Phillips, 2003). The Ethics Committee of the Dental Medicine Faculty of Damascus University approved the research protocol. The data were statistically analysed using Student’s t-test. A level of statistical signiﬁcance of 0.05 was assumed. The statistical software SPSS version 13.0 was used for data analysis.
2. Materials and methods Twenty strip patterns (3 · 10 · 60 mm) were made of dental modelling wax (Tenatex Red, Kemdent, UK). Moulds were made by placing the wax patterns in a metal ﬂask with a dental stone (Bego, Germany). The lower half of the ﬂask was ﬁlled with mixed dental stone, a glass slab was placed on the surface, and the dental stone was allowed to set. Four wax patterns were placed on the glass slab and fastened with an adhesive. The stone surface was painted with a separating medium (Die Bub, JIM Neg Col. Bloomﬁeld, CT, USA). The upper half of the ﬂask was placed over the lower half, ﬁlled with mixed dental stone, and allowed to set. The halves of the ﬂask were separated, the wax patterns were removed, and the stone surface was painted with separating medium. The high-impact acrylic resin Lucitone 199 (Dentsply International Inc., Degu Dent GmbH, Hanau, Germany) and the traditional acrylic resin Rodex (SPD, Italy) were mixed according to the manufacturers’ instructions and packed during the dough stage into the moulds. The halves of the ﬂask were clamped. The recommended polymerization cycles were followed for each material. Each material was cured by placing the ﬂask in a water bath at 72 C for 1 h, followed by 100 C for 30 min. The ﬂask was left in the water overnight before removal. Specimens were ﬁnished with 320-grit sandpaper (Rados, Morocco) and a tungsten carbide bur (Strong 204, Microtower, Korea) at 4000 rpm, and stored in artiﬁcial saliva at 37 C for 2 weeks. The specimens were subjected to the three-point ﬂexural strength test (Fig. 1). Force was applied by a Testometric M350-5CT (Rochdale, England) (Fig. 2) with Win Test software and a 500-kg load cell at a crosshead speed of 5 mm/min. The span length was 46 mm. The ﬂexural strength (FS, in MPa) was calculated by FS = 3PL/2 bd2, where P is the maximum load (N), L is the span length (m), b is the specimen width
Strip resin specimen during 3-point ﬂexure test.
The testing machine (Testometric).
Elastic modulus and ﬂexural strength comparisons of high-impact and traditional denture
Table 1 Mean, standard deviation, minimum and maximum values of elastic modulus (MPa) and ﬂexural strength (MPa) for the two types of acrylic resins. Material
Elastic modulus Flexural strength Elastic modulus Flexural strength
1229.68 82.43 1602.68 69.77
38.82 6.85 37.18 7.31
1177.4 66.937 1530.9 58.924
1304.9 89.027 1667.2 82.792
Independent sample T-test results.
Std. error diﬀerence
Elastic modulus (Mpa) Flexure strength (Mpa)
The mean difference is signiﬁcant (P < .05).
3. Results Table 1 presents the descriptive statistics of the elastic modulus and ﬂexural strength for Lucitone 199 and Rodex. The high-impact resin material (Lucitone 199) exhibited a lower mean elastic modulus and a higher mean ﬂexural strength compared to the traditional resin material (Rodex) (p = .000 and .001, respectively, by Student’s t-test; Table 2).
4. Discussion A denture base material with a high elastic modulus can withstand permanent mastication-induced deformation. Fracture of the upper dentures invariably occurs through the midline of the denture, due to ﬂexure. Therefore, the denture base should have sufﬁcient ﬂexural strength to resist fracture (McCabe and Walls, 1998). This study compared the elastic modulus and ﬂexural strength between high-impact and traditional denture base acrylic resins. The experimental circumstances were similar to those of the clinical situation. Specimens were 60 mm in length, similar to the width of the upper denture between the two molars (Stafford et al., 1982), and the specimen thickness (3 mm) was similar to that of the denture. After immersion in artiﬁcial saliva at 37 C for 2 weeks, the mean elastic modulus of the high-impact resin (Lucitone 199, 1229.68 MPa) was signiﬁcantly lower than that of the traditional resin (Rodex, 1602.68 MPa). The elastic modulus reﬂects the stiffness of a material (Craig et al., 2004). Therefore, the high-impact resin exhibited less stiffness than the traditional resin. O’Brien (1997) mentioned that the inclusion of rubber in the high-impact resin improved the impact strength but reduced the stiffness, which might help explain the lower elastic modulus of the high-impact resin. This result is in agreement with Meng and Latta (2005), who found that Lucitone 199 exhibited the lowest elastic modulus when compared to two traditional resins (ProBase Hot, Sledgehammer Maxipack). The mean ﬂexural strength of the high-impact resin (Lucitone 199, 82.43 MPa) was signiﬁcantly higher than that of the traditional resin (Rodex, 69.77 MPa). During the three-point ﬂexure test, compressive stresses were generated at the middle of the upper surface of the tested strip, whereas tension stresses were generated at the lower surface (Manappallil, 2003). Fracture of
the strips occurred due to the gradual propagation of small cracks at the sites of tension on the lower surface (Kaine et al., 2000). According to O’Brien (1997), the inclusion of rubber in highimpact resin had a craze-inhibiting effect, which could explain the increased ﬂexural strength of Lucitone 199. Diaz-Arnold et al. (2008) and Meng and Latta (2005) reported mean values for the ﬂexural strength of Lucitone 199 of 83.97 and 99.5 MPa, respectively. The ﬂexural strength is related to the distance between the two supporting bars, test speed, and dimensions (width and thickness) of the tested strip (Anusavice and Phillips, 2003). These aspects differed in the present study compared to previous studies, which might explain the difference in the ﬂexural strength values among the different studies. Meng and Latta (2005) found that the ﬂexural strength of high-impact Lucitone 199 was higher than those of two traditional resins (ProBase Hot, Sledgehammer Maxipack). However, Diaz-Arnold et al. (2008) found no signiﬁcant difference between the ﬂexural strength of Lucitone 199 compared to three heat-cured acrylic resins (Diamond D, Fricke HI-I, Nature-Cryl Hi-Plus). 5. Conclusion The high-impact acrylic resin (Lucitone 199) exhibited less stiffness and, therefore, greater deformation compared to the traditional acrylic resin (Rodex). The high-impact resin also showed greater ﬂexural/fracture strength than the traditional acrylic resin. Within the limitations of this study, it can be concluded that the high-impact acrylic resin is a suitable denture base material for patients who are suffering from clinical fracture of the acrylic denture. Conﬂict of interest The current research is free of conﬂict of interest.
Acknowledgment The authors would like to thank Damascus University for the ﬁnancial support of the study.
18 Appendix A. See Tables 1 and 2. References Anusavice, K.J., Phillips, R.W., 2003. Phillips’ Science of Dental Materials, 11th ed. WB Saunders, St. Louis, pp. 83–89. Cheng, Y.Y., Cheung, W.L., Chow, T.W., 2010. Strain analysis of maxillary complete denture with three-dimensional ﬁnite element method. J. Prosthet. Dent. 103, 309–318. Craig, R.G., Powers, J.M., Wataha, J.C., 2004. Dental Materials, Properties and Manipulation, 8th ed. Mosby, St. Louis, p. 24. Diaz-Arnold, A.M., Varags, M.A., Shaull, R.L., Laffoon, J.E., Oian, F., 2008. Flexural and fatigue strengths of denture base resin. J. Prothet. Dent. 100, 47–51. Hirajima, Y., Takahashi, H., Minakuchi, S., 2009. Inﬂuence of a denture strengthener on the deformation of a maxillary complete denture. Dent. Mater. 28, 507–512.
N.M. Ajaj-ALKordy, M.H. Alsaadi Johnston, E.P., Nicholls, J.I., Smith, D.E., 1981. Flexure fatigue of 10 commonly used denture base resins. J. Prosthet. Dent. 46, 478–483. Kaine, T., Fujii, K., Arikawa, H., Inoue, K., 2000. Flexural properties and impact strength of denture base polymer reinforced with woven glass ﬁber. Dent. Mater. 16, 150–158. Kelly, E., 1969. Fatigue failure in denture base polymers. J. Prosthet. Dent. 21, 257–266. Manappallil, J.J., 2003. Basic Dental Materials, second ed. Jaypee Brother Medical Publishers, New Delhi, p. 16. McCabe, J.F., Walls, A.W.G., 1998. Applied Dental Materials, 8th ed. Blackwell Science, Oxford, p. 97. Meng, T.R., Latta, M.A., 2005. Physical properties of four acrylic denture base resins. J. Contemp. Dent. Pract. 6, 93–100. O’Brien, W.J., 1997. Dental Materials and Their Selection, Second ed. Quintessence Publishing Co., Inc., pp. 86–94. Seo, R.S., Murata, H., Hong, G., Vergani, C.E., Hamada, T., 2006. Inﬂuence of thermal and mechanical stresses on the strength of intact and relined denture bases. J. Prosthet. Dent. 96, 59–67. Stafford, G.D., Lewis, T.T., Huggett, R., 1982. Fatigue testing of denture base polymers. J. Oral. Rehabil. 9, 139–154.